HEAT TREATMENT PROCEDURE QUALIFICATION
HEAT TREATMENT PROCEDURE QUALIFICATION
HEAT TREATMENT PROCEDURE QUALIFICATION Final Technical Report The Pennsylvania State University University Park, PA Work Performed Under Contract No. DE-FC07-99ID13841 Work Prepared for U.S. Department of Energy
ii This material is based upon work supported by the U.S. Department of Energy under Award No. DE-FC07-99ID13841 Any opinions, findings, and conclusions or recommendations expressed in this material are those of the authors and do not necessarily reflect the views of the Department of Energy DISCLAIMER This report was prepared as an account of work sponsored by an agency of the United States Government.
Neither the United States Government nor any agency thereof, nor any of their employees, make any warranty, express or implied, or assumes any legal liability or responsibility for the accuracy, completeness, or usefulness of any information, apparatus, product, or process disclosed, or represents that its use would not infringe privately owned rights. Reference herein to any specific commercial product, process, or service by trade name, trademark, manufacturer, or otherwise does not necessarily constitute or imply its endorsement, recommendation, or favoring by the United States Government or any agency thereof.
The views and opinions of authors expressed herein do not necessarily state or reflect those of the United States Government or any agency thereof.
This report has been reproduced directly from the best available copy.
iii Table of Contents 1.0 Introduction … … 1 2.0 Evaluation of Heat Treatment Practices in Steel Foundries … . 6 2.1 Austenitizing of Carbon & Low Alloy Steels … … 6 2.1.1 Austenitizing Temperature . . 6 2.1.2 Austenitizing Time … … 8 2.1.3 Furnace Characteristics … … 11 2.1.4 Furnace Loading . . 13 2.1.5 Extent of Austenitization … … 19 2.2 Solutionizing of High Alloy Steels . … 20 2.3 Quenching of Carbon and Low Alloy Steels … … 21 2.3.1 Quenchant Characteristics . … 21 2.3.2 Quench Tank Loading Effects .
. 25 2.3.3 Quench Delay … … 29 2.3.4 Normalizing of Carbon & Low Alloy Steels . … 29 2.3.5 Quenching/cooling of High Alloy Steels … … 30 2.3.6 Pre-qualification of High Alloy Steels Using HTPQ Ratings … … 32 2.4 Hardenability of Carbon & Low Alloy Steels … … 35 2.4.1 Hardenability Concepts … … 35 2.4.2 Use of Hardenability Concepts for Heat Treatment Procedure Qualification of Carbon & Low Alloy Steels … … 38 2.4.3 Hardenability Concepts for HTPQ of Carbon and Low Alloy Steels— An Example … … 42 2.4.4 Alternate HTPQ scheme based on Quenched Hardness … … 44 2.5 Tempering of Carbon & Low Alloy Steels … … 47 2.5.1 Tempering Time and Temperature … … 47 2.5.2 Comparison of Tempering Models … … 52 2.5.3 Effects of Furnace Loading & Section Size … .
55 2.5.4 Extent of Tempering Estimates … . 56 2.6 Perspectives on Heat Treatment Specifications … … 57 2.6.1 Heat Treatment Specifications . … 57 2.6.2 Furnace Temperature Uniformity and Control … … 59 2.6.3 Existing Qualification Guidelines within Current Heat Treatment Specifications [ASTM 370-97A . . 61 3.0 Summary . … 62 4.0 References . . 65 Appendix A: Extent of Heat Treatment … … 67 Appendix B: Standard Practice for Qualification of Heat Treatment Procedures for Carbon and Low Alloy Steel Castings … … 71 Appendix C: Standard Practice for Qualification of Heat Treatment Procedures for Nickel-Base and High Alloy Steel Castings … … 82
iv Tables and Figures Table I: Comprehensive heat treatment variable list … … 4 Table II: Critical heat treatment procedure qualification variables . … 5 Table III: Recommended Austenitizing Temperatures for Wrought Carbon and Low Alloy Steels . . 7 Table IV: Comparison of required, recommended, and typically used austenitization temperatures for 1030 and 8630 type steels … … 8 Table V: Austenitizing temperature ranges reported by SFSA member foundries for carbon and low alloy steels … … 8 Table VI: Summary of austenitizing practices used by SFSA member foundries … … 9 Table VII: Time required for complete austenitization of cast steels at various austenitizing temperatures … … 10 Table VIII: Summary of PSU short cycle heat treatment studies in a heavily loaded laboratory furnace … … 19 Table IX: Expected Grossman numbers and film coefficients for water during quenching … … 23 Table X: The effect of water temperature on cooling rates and film coefficients in 1.5in diameter 4130 steel bars water quenched from 1550F … … 23 Table XI: Survey Responses from SFSA Member Foundries for Austenitic Grades .
… 32 Table XII: Survey Responses from SFSA Member Foundries for Duplex Grades . . 33 Table XIII: Survey Responses from SFSA Member Foundries for Ferritic Grades . . 33 Table XIV: Survey Responses from SFSA Member Foundries for Martensitic Grades . . 33 Table XV: Survey Responses from SFSA Member Foundries for Superaustenitic Grades . … 34 Table XVI: Survey Responses from SFSA Member Foundries for Nickel Grades . … 34 Table XVII: Individual alloying element hardenability factors (DI Factors) used for overall alloy DI calculation … … 37 Table XVIII: Steel alloy DI based on the sum of individual alloy factors from Table XVII … … 38 Table XIX: Example composition of 8625 steel … … 42 Table XX: Minimum quenched hardness values for acceptable HTPQ of carbon and low alloy steels based on alloy carbon content … … 47 Table XXI: Tempered hardness variations due to tempering temperature variations for 8630 steel of nominal composition.
Estimated with the Creusot Loire tempering model [MAYN1978]. The tempering temperature is 1150F . … 51
v Table XXII: Comparison of tempering model characteristics . … 52 Table XXIII: 8630 steel compositions used for tempered hardness calculations using the Creusot-Loire tempering model . . 53 Table XXIV: Calculated quenched & tempered hardness for 8630 steels tempered for 4 hours at various temperatures using the Creusot-Loire tempering model … … 53 Table XXV: Calculated quenched & tempered hardness for 8630 steels tempered at 1100F for various hold times using the Creusot-Loire tempering model … … 54 Table XXVI: List of Standards and Specifications with reference to Heat Treatment of Steel Castings.…58 Table XXVII: Limits on temperature uniformity in furnaces … … 59 Table XXVIII: Allowable variations from set-point temperatures … … 59 Table XXIX: Hold times for annealing, normalizing, and austenitizing based on section size in AMS 2759 1c … … 60 Table XXX: Permissible operating temperature conditions for quenchants … … 60 Figure 1: Volume percent austenite formed from pearlite in a eutectoid steel as a function of time at an austenitizing temperature of 1380F .
… 8 Figure 2: Effect of austenitizing temperature on the rate of austenite formation from pearlite in a eutectoid steel … … 9 Figure 3: Comparison of Charpy V-notch impact energy as a function of temperature for standard and short cycle austenitization treatments, quenched & tempered plain carbon steel … … 10 Figure 4: Time-Temperature profiles for 3.0, 5.0, and 8.0 inch section sizes during an austenitizing test. Thermocouples were placed on the surface and at the center of each test block … … 11 Figure 5: Heating rates of 6.0 inch sections of CrMo and MnNiCrMo cast steels in a 1750F production furnace … … 12 Figure 6: Heating of 1.0 inch sections of MnCrMo and MnB cast steels in an experimental furnace at 1750F … … 12 Figure 7: Heating of 3.0 inch sections of MnCrMo and MnB cast steels in an experimental furnace at 1750F … … 13 Figure 8: Temperature response of loaded heat treatment furnaces during austenitizing … … 15 Figure 9: Time for heating to 250C in a convection furnace.
Specimen size 50mm diameter x 100mm, 1 and 15 specimens respectively … … 16 Figure 10: Time for heating to 250C in a convection furnace. Specimen size 150mm diameter x 300mm. 1 specimen and 4 specimens, Respectively … … 16 Figure 11: Dependence of overall heating time on initial furnace temperature for a convection furnace. Specimen size 150mm diameter x 300mm. 2 specimens … … 17 Figure 12: Heat-up time in an electric muffle furnace for a die block measuring 2300 x 950 x 500mm (Dimensions of furnace: 6500 x 1400 x 1100mm … … 18
vi Figure 13: Effect of quench bath temperature on heat removal using a Wolfson probe. (water quenchant; velocity of 50ft/min … … 22 Figure 14: Analysis of cooling curve data during quench severity studies of water quenchants … . 24 Figure 15: The effect of end-quench water temperature on the resultant hardness of Jominy end-quench bars … … 25 Figure 16: Variation of quenching cooling curve performance at the center of casting loads at various packing densities for a water quenchant . . 26 Figure 17: The effect of steel mass and section size on the cooling rates of steel sections quenched in hot water without agitation .
… 28 Figure 18: Still air quenching at the center of plain carbon steel bars … … 29 Figure 19: TTT diagrams of 25%Cr-16%Mn-.54% ferritic-austenitic stainless steel in ferrite (a) and austenite (b … … 31 Figure 20: Calculated and experimental Jominy hardness values for AISI 4130 steel austenitized and quenched from 1575F. Curves A, B, C were calculated from DI values; curve D was obtained from measured hardness values … … 35 Figure 21: Fundamental relationship among ideal critical diameter, actual critical diameter, and severity of quenching … … 39 Figure 22: Relationship between ideal critical diameter and the critical thickness that can be fully hardened using a quenching medium with quench severity H .
… 39 Figure 23: Plots of DI (inches) versus equivalent casting section diameter for prequalification schema….40 Figure 24: Schematic representation of HTPQ “acceptable and pre-qualified” regions based on hardenability concepts for carbon and low alloy steels … … 41 Figure 25: Effective HTPQ Quench Severity Values as a function of overall alloy DI and the HTPQ section thickness. Successful HTPQ at an effective HTPQ quench severity value prequalifies other alloy (DI) and section size combinations with equal or lower effective HTPQ quench severity values . . 41 Figure 26: Effective HTPQ Quench Severity Values as a function of overall alloy DI and the HTPQ diameter.
Successful HTPQ at an effective HTPQ quench severity value prequalifies other alloy (DI) and section size combinations with equal or lower effective HTPQ quench severity values … … 42 Figure 27: Example alloy DI factors for an 8625 steel. The sum of the alloy factors is 1.3994. (.1929 + .5437 + .3403 + .0795 + .2430 = 1.3994 … … 43 Figure 28: Alloy DI determination for an 8625 steel … … 43 Figure 29: Prequalified DI and section thickness combinations for an 8625 steel. All combinations represented by values upwards and to the left of the bounding lines are pre-qualified … … 44 Figure 30: Hardness of martensite as a function of carbon content .
… 45 Figure 31: Hardness of martensite as a function of carbon content. The blue band represents commonly achieved industry values … … 45
vii Figure 32: As-quenched hardness as a function of carbon content of martensite. The gray field represents commonly achieved industry values; the blue and gold lines represent 95% and 90% martensite, respectively. The red line is the recommended minimum quenched hardness for HTPQ Method C … … 46 Figure 33: Tempering response of a wrought SAE 4340 steel for quench & temper heat treatments……48 Figure 34: Mechanical properties of a 4340 wrought steel oil quenched to produce a martensitic structure and tempered for 1 hour at various tempering temperatures … … 49 Figure 35: Quenched & tempered hardness as a function of carbon content for iron-carbon alloys tempered at various temperatures … … 50 Figure 36: Calculated variation in quenched & tempered hardness as a function of tempering time at 1100F for three compositions of 8630 steel … … 54 Figure 37: Calculated variation in quenched & tempered hardness as a function of tempering temperature for three compositions of 8630 steel tempered for four hours .
. 55 Figure 38: Tempering response for 1- and 3-inch sections of C-Mn cast steel heated to 1250F in an experimental furnace … … 56
1 Heat Treatment Procedure Qualification for Steel Castings Abstract Heat treatment practices used by steel foundries have been carefully studied as part of comprehensive heat treatment procedure qualification development trials. These studies highlight the relationships between critical heat treatment process control parameters and heat treatment success. Foundry heat treatment trials to develop heat treatment procedure qualifications have shed light on the relationship between heat treatment theory and current practices. Furnace load time-temperature profiles in steel foundries exhibit significant differences depending on heat treatment equipment, furnace loading practice, and furnace maintenance.
Time-temperature profiles of furnace control thermocouples can be very different from the time-temperature profiles observed at the center of casting loads in the furnace. Typical austenitization temperatures and holding times used by steel foundries far exceed what is required for transformation to austenite. Quenching and hardenability concepts were also investigated. Heat treatment procedure qualification (HTPQ) schema to demonstrate heat treatment success and to pre-qualify other alloys and section sizes requiring lesser hardenability have been developed. Tempering success is dependent on both tempering time and temperature.
As such, furnace temperature uniformity and control of furnace loading during tempering is critical to obtain the desired mechanical properties. The ramp-up time in the furnace prior to the establishment of steady state heat treatment conditions contributes to the extent of heat treatment performed. This influence of ramp-up to temperature during tempering has been quantified.
Project Team Debo Aichbhaumik, DOE Golden Field Office Malcolm Blair, SFSA Harvey Wong, DOE HQ Penn State University Research Mariol Charles Nicholas Deskevich Vipin Varkey Robert Voigt, PI Angela Wollenburg 1.0 Introduction Principles of heat treatment for steels have been well-studied and are well-understood. These principles provide the basis for heat treatment specifications and practices used by heat treaters and steel foundries on a daily basis. While current heat treatment specifications provide general guidelines for the heat treatment of steel castings, they do not address all critical aspects of steel casting heat treatment practice.
A wide range of heat treatment equipment and heat treatment control strategies are used in today’s steel foundries. Modern temperature data acquisition systems allow increased knowledge of the thermal conditions in a furnace load, not just in the furnace itself. This improvement in technology affords the possibility of load-based heat treatment time and temperature cycles, which are more precise than heat treatment cycles based on furnace temperature. Challenges in temperature monitoring of loaded furnaces have
2 led to overly conservative practices to ensure complete heating of casting loads. Commonly used “hour-per-inch” rules are used to ensure that the centers of casting loads in heat treatment furnaces reach the appropriate temperature. However, these practices often result in holding castings at temperature far longer than is necessary. For example, current heat treatment specifications for high alloy steels prescribe only the minimum heat treating temperatures and the quenching media. Variations in furnace conditions, furnace loading, quench delay, quench tank temperature, and quenchant velocity are not addressed in the current specifications.
However, it is clear that these parameters must be carefully controlled to develop a successful heat treatment practice. The use of heat treatment procedure qualification (HTPQ) methodologies can lead to the development of foundry-specific heat treatment practice guidelines to ensure heat treatment success over the broad range of heat treatment conditions that are likely to occur in a given foundry. Toward this aim, fully instrumented comprehensive HTPQ development trials have been conducted at three steel foundries. These in-plant trials and complementary Penn State laboratory heat treatment trials have served to assess the degree of heat treatment process control required for assurance of heat treatment success.
Current heat treatment practices used by steel foundries for carbon, low alloy and high alloy steels have been critically assessed based on the heat treatment literature, comprehensive HTPQ development trial results from steel foundries, and laboratory heat treatment trials. The applicability of heat treatment models from the literature has been assessed. From this assessment, critical components of steel casting heat treatment practice success have been identified. Also, robust HTPQ guidelines useful to both foundries and steel casting customers have been developed.
Heat treatment science is the basis from which most, if not all, of current heat treatment practices used in the steel foundry industry have been developed.
However, a direct link between heat treatment science and practice often cannot be developed. For example, it is difficult, if not impossible, to link the kinetics of the ferrite to austenite transformation to a precise recommendation for furnace ramp-up and hold times during austenitizing of low alloy steel castings. Similarly, it is difficult to link austenite to martensite transformation kinetics information to precise recommendations for the minimum and maximum quench delays when transferring a basket of complex geometry castings into a quench tank. As a consequence, the need to develop robust heat treatment procedure qualification methods to ensure adequate heat treatment process control is paramount.
Penn State surveys have shown that significant differences exist in the current heat treatment practices used by SFSA member foundries. While most steel foundries use “hour-per-inch” guidelines to establish proper heat treatment times, the practice of this rule varies between foundries. For example, some foundries specify a fixed time in the furnace for their heat treatments. In this scenario, load variations can contribute to variations in actual ramp up times that result in significant variations in heat treatment hold times from load to load. Other heat treaters instrument the load itself during ramp up and use the temperature of the load to establish a sufficient heat treatment hold time.
Critical issues such as this must be fully addressed before adopting short cycle heat treatments, which have been successful in some steel foundries but are not widely used [BRIG1958].
Heat treatment procedure qualification (HTPQ) methodologies offer the opportunity to develop robust heat treatment practices based on both fundamental principles and foundry-specific heat
3 treatment practices. The comprehensive in-plant HTPQ development trials that are the foundation of this Penn State/SFSA research therefore serve two main purposes: 1. To develop simple robust HTPQ guidelines that can be used by foundries and casting customers for heat treatment quality assurance, and 2. To develop stronger links between fundamental heat treatment science and steel foundry heat treatment practice that can lead to better specification of heat treatment control limits.
Table I lists the key heat treatment process, practice and equipment variables that can be expected to influence heat treatment response. Process and equipment variables affect heat treatment response as do the selection of appropriate HTPQ set-points. Some of these key heat treatment response variables, such as the chemical composition and geometry, are inherent to the casting itself. For example, a low alloy composition has a lower hardenability, which requires a more aggressive quench to achieve full hardness when compared to richer alloy compositions. Furnace air circulation and quenchant circulation are dependent on the casting geometry.
The “ranginess” or “compactness” of a casting can also affect the packing density of the heat treatment load.
Heat treatment equipment such as the furnace size and type can vary from foundry to foundry and can also vary from furnace to furnace within a foundry. The condition of the furnace door seal and the furnace insulation type strongly influences the time and temperature response of a furnace [CONN2001]. The time and temperature response of a furnace can also depend on the furnace controller. Temperature ramp-up is controlled either by the overall furnace capacity and load or by the furnace controller itself. Furthermore, the control of the furnace can also be affected by the type and location of the control thermocouple.
4 Table I: Comprehensive heat treatment variable list Heat Treatment Variable Possible HTPQ Consideration Casting Grade Grade/or Composition Composition Grade/Composition Min. Section Size Not Significant Max. Section Size Max. Section Size Weight Max. Section Size Compactness/ Ranginess Max. Section Size Microstructure Not Significant Weld Repair Not Significant Prior Heat Treatment Not Significant Surface Condition Not Significant Heat Treatment Equipment Furnace Type Heat Treatment Time and Temperature Furnace Size Heat Treatment Time and Temperature Burner Location Heat Treatment Time and Temperature No.
of Burners Heat Treatment Time and Temperature Insulation Heat Treatment Time and Temperature Burner Operating Characteristics Heat Treatment Time and Temperature Refractory Supports Heat Treatment Time and Temperature Door Seal Type Heat Treatment Time and Temperature Door Seal Condition Heat Treatment Time and Temperature Furnace Control Heat Treatment Time and Temperature Ramp-up Control Heat Treatment Time and Temperature Zone Control Heat Treatment Time and Temperature Cool-down Control Heat Treatment Time and Temperature Control T/C Location Heat Treatment Time and Temperature Control T/C Response Heat Treatment Time and Temperature Atmosphere Not Significant Hold Temperature Variation Heat Treatment Time and Temperature Heat Treatment Variable Possible HTPQ Consideration Heat Treatment Practice Set Temperature Heat Treatment Temperature Load Temperature Heat Treatment Temperature Ramp-up Time Heat Treatment Time Hold Time Heat Treatment Time Basket / Rack Geometry Full load condition Weight of Load Full load condition Density of Load Full load Condition Load Location Full Load Condition Initial Furnace Temperature Heat Treatment Time and Temperature Ramp / Hold Time Criteria Heat Treatment Time and Temperature Hold Time Variation Heat Treatment Time Quenching Equipment Quenchant Type Quenchant Type Tank Volume Initial Quench Temperature Make-up Water Conditions Initial Quench Temperature Pump Inlet / Outlet Locations Initial Quench Temperature Quench Practice / Control Quench Velocity Quench Velocity Delay Time Delay Time Initial Quench Temperature Initial Quench Temperature Initial Load Temperature Not Significant Load Volume Full Load Condition Load Surface Area Full Load Condition Quenched Hardness Minimum As-Quenched Hardness Final Casting Temperature Final Quench Temperature Casting Surface Condition Not Significant Localized Quench Velocity Quench Velocity Localized Quench Temperature Final Quench Temperature Normalizing Ambient Temperature Not Significant Air Velocity Air Velocity Air humidity (relative) Less Significant Load Volume Full Load Condition Load Density Full Load Condition Localized Air Velocity Air Velocity Localized Temperature Air
5 Ultimately, it is the time and temperature response of the heat treated castings rather than the time and temperature of the furnace that controls treated properties. The “extent of heat treatment” includes not only time-at-temperature but also includes a component of the time-to- temperature, furnace ramp-up. This extent of heat treatment is different for different section sizes in a complex casting and for different castings within the heat treatment load. Castings in the center of a heat treatment basket in fully loaded furnaces can be expected to have significantly different time-temperature profiles than castings that are fully exposed in partially loaded furnaces.
The quenching system affects the ability of the heat treater to cool the casting uniformly and quickly. The effective quench severity experienced by a casting is influenced by many factors. The tank volume and quenchant type are critical. Make-up water to control temperature increases in the tank, as well as local quenchant velocities, influence the casting cooling rates. Quenching practice is as important as the quenching equipment. The delay time from the furnace to the quench tank must be short enough to prohibit unwanted microstructure transformations. The quench load size, density and casting surface condition will affect the local heat transfer coefficient at the casting-quenchant interface.
A successful HTPQ strategy incorporates critical heat treatment equipment, process and practice variables into a fundamental qualification framework without placing limits on less significant variables. It relies on demonstration of heat treatment success for HTPQ test conditions that mimic heat treatment process variable ranges commonly observed during production heat treatment. From the very long list of heat treatment variables shown in Table I comes a much shorter list of the most critical heat treatment parameters that need to be quantified as part of a robust HTPQ guideline. This shorter list of critical HTPQ variables is shown in Table II.
Table II: Critical heat treatment procedure qualification variables All Heat Treatments • Alloy grade/composition • Maximum casting section size • Time-temperature profile during heat treatment • Furnace loading at full load condition Additional Quench & Temper Heat Treatment Considerations • Quenchant type • Initial quench tank temperature • Quench tank velocity • Final quench tank temperature after quenching Additional Normalizing Heat Treatment Considerations • Air velocity during cooling For the purposes of HTPQ development, many critical heat treatment variables can be adequately expressed by considering their effects on load thermocouple time and temperature profiles.
Together, heat treatment time and temperature express the amount of energy imparted to the heat treated casting. Within limits, time and temperature during heat treatment are interchangeable, i.e., a longer heat treatment at a lower temperature can impart the same extent of heat treatment as shorter heat treatment at a higher temperature. This equivalence can be expressed using an “extent of heat treatment” term, E, that will be developed later in this